CHAPTER 1. BACKGROUND
1.2 INTERCONNECT SCALING ISSUES
1.2.2 Technological issues of interconnects scaling
11 because of the less tendency of cobalt to diffuse with respect to copper. This fact is due to the dependency of metals diffusivity on melting temperature (Tm) and crystal structure .
First, cobalt Tm is higher than copper Tm, implying a greater activation energy required for diffusion. Secondly, as regards the crystal structure, transmission electron microscope images have revealed that nanometric cobalt presents bamboo grains that copper loses when scaled down below 90 nm ; this bamboo-grains structure (which consists of crystallites that expand across the entire width of the interconnect and are aligned in the direction of current flow) plays a critical role in retarding diffusion. In a few words, cobalt diffusivity is smaller than copper one (DCo < DCu) leading, by virtue of equation 1.3, to a smaller electromigration-induced current density (JEM,Co < JEM,Cu), thus cobalt proves to have better electromigration reliability.
However, it is worth to highlight that despite the benefits cobalt could provide, it would not replace copper entirely but just in the first layers, where there are local interconnects and dimensions at stake are very small (in the order of few dozens of nanometers) . For global interconnects, that run longer distances and are more detached from each other, it makes sense to continue using copper, and this is the reason why it will be investigated in this thesis work as well as cobalt.
12 by light and the developer will dissolve it away, leaving behind a coating in the masked areas3.
2) Etching, in order to create the hole of the VIA.
Figure 1.5: general fabrication method of a Vertical Interconnect Access. (a) Lithography; (b) etching;
(c) photoresist removal; (d) deposition of TaN barrier and Ta liner; (e) filling with metal;
(f) chemical mechanical polishing .
3The previous explanation concerns the use a positive photoresist. In the case of a negative photoresist the organic material in the unmasked areas will be strengthened by light (because of either polymerization or cross-linking) and the developer will dissolve away the regions which did not undergo light exposure.
13 3) Photoresist removal, to take away the light sensitive organic material used in the
4) Deposition of TaN barrier layer and Ta liner, whose functions have been already discussed in the previous paragraph.
5) Filling of the hole with conductive metal, to create the Vertical Interconnect Access.
(This is a two-step process: first a nucleation layer is deposited, usually by chemical vapor deposition, then the bulk layer is formed, typically by electrochemical deposition)
6) Chemical mechanical polishing, for removing the excess of metal from the wafer surface.
With downscaling, the rising challenge is not only fabricating smaller components, but also make them align properly when they need to be stacked one above the other; considering the VIA fabrication explained above, it’s easy to understand that this task should be theoretically fulfilled by lithography.
The effectiveness of photolithography depends on the alignment of the substrate to be processed with respect to the mask used in the optical exposure. Unfortunately, misalignments always occur, due to various causes. The maximum error in alignment is called edge placement error, usually indicated with the acronym EPE; EPE should be smaller than one-fourth of the critical dimension .
In the case of the Vertical Interconnect Access, alignment errors entail a reduction of the section in contact with the underlying metallic layer, with a consequent increase in resistivity and a deterioration of performance.
The need for eliminating the edge placement errors of top-down processing has led to an increasing demand for development of bottom-up approaches, which enable self-alignment and avoid going through the numerous steps of traditional (top-down) nanopatterning techniques.
One of such bottom-up approaches, that has gained more and more attention in the last two decades, is the area selective atomic layer deposition (AS-ALD).
ALD is a deposition technique which allows to grow thin films on solid surfaces in a bottom-up fashioned way, building them bottom-up layer-by-layer, with promising and unique capabilities for sub 45 nm CMOS technology .
14 A deposition technique is said area-selective when it aims to limit the deposition to some specific areas of interest, in such a way that the substrate is prevented to be fully coated.
The locations where the deposition should and should not take place are usually referred to as growth and non-growth areas respectively.
The disruptive potential of AS-ALD in aligning two materials on top of each other is shown in figure 1.6, where there is a comparison with a conventional patterning pathway which makes use of lithography and etching . Both ALD and area-selectivity, however, will be thoroughly discussed in chapter 2.
Figure 1.6: (a) conventional patterning pathway, which consists of film deposition, lithography and etching;
(b) area-selective atomic layer deposition, that enables self-alignment by making the deposition occur only where it is required .
The edge placement error is not the only problem that arises during VIA fabrication. During the filling of the VIA, in fact, the usage of traditional top-down deposition techniques may provoke the formation of defects, which obviously deteriorate the properties of the metal .
The most common examples of such defects are the so-called voids and seams, which are respectively represented in figure 1.7 (b) and (c). Basically, both voids and seams are gaps which develop as result of incomplete/irregular filling, interrupting the continuity of the
15 metal; the only difference between voids and seams is the shape of the gap, which is in any case located in the center of the VIA channel.
Once again, the usage of a bottom-up approach could be the solution to the problem: the area selective ALD technique turns out to be the right strategy to not simply mitigate, but even eliminate the incomplete filling defects, since it builds structures layer-by-layer and permits to reach a good fill, like shown in fig 1.7 (a).
Figure 1.7: VIA filling.
(a) Good VIA filling; (b) void formation during VIA filling; (c) seam formation during VIA filling .